#------------------------------------------------------------------------------
#$Date: 2019-11-23 04:49:39 +0200 (Sat, 23 Nov 2019) $
#$Revision: 232164 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/34/70/4347093.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4347093
loop_
_publ_author_name
'Roy, Soumyabrata'
'Sarkar, Sumanta'
'Pan, Jaysree'
'Waghmare, Umesh V.'
'Dhanya, R.'
'Narayana, Chandrabhas'
'Peter, Sebastian C.'
_publ_section_title
;
 Crystal Structure and Band Gap Engineering in Polyoxometalate-Based
 Inorganic-Organic Hybrids.
;
_journal_issue                   7
_journal_name_full               'Inorganic chemistry'
_journal_page_first              3364
_journal_page_last               3377
_journal_paper_doi               10.1021/acs.inorgchem.5b02718
_journal_volume                  55
_journal_year                    2016
_chemical_formula_moiety         'Mo12 O40 Si, 2(H2 O), 2(C10 H10 N2)'
_chemical_formula_sum            'C20 H24 Cl0 Cu0 Mo12 N4 O42 Si'
_chemical_formula_weight         2171.80
_chemical_name_common            '[(H4SiMo12O40)][(C10H8N2)2].2H2O'
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2yn'
_space_group_name_H-M_alt        'P 1 21/n 1'
_atom_sites_solution_hydrogens   mixed
_audit_creation_date             2016-01-28
_audit_creation_method
;
Olex2 1.2-beta
(compiled 2015.01.19 svn.r3143 for OlexSys, GUI svn.r4992)
;
_cell_angle_alpha                90
_cell_angle_beta                 103.319(2)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   11.5292(4)
_cell_length_b                   12.0812(5)
_cell_length_c                   17.3184(7)
_cell_measurement_reflns_used    4087
_cell_measurement_temperature    295(2)
_cell_measurement_theta_max      25
_cell_measurement_theta_min      2.6
_cell_volume                     2347.34(16)
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2008)'
_diffrn_ambient_temperature      295.15
_diffrn_measured_fraction_theta_full 0.989
_diffrn_measured_fraction_theta_max 0.989
_diffrn_measurement_device_type  'Smart X2 APEX II CCD'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0622
_diffrn_reflns_av_unetI/netI     0.0473
_diffrn_reflns_Laue_measured_fraction_full 0.989
_diffrn_reflns_Laue_measured_fraction_max 0.989
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_limit_l_min       -20
_diffrn_reflns_number            23967
_diffrn_reflns_point_group_measured_fraction_full 0.989
_diffrn_reflns_point_group_measured_fraction_max 0.989
_diffrn_reflns_theta_full        24.996
_diffrn_reflns_theta_max         24.996
_diffrn_reflns_theta_min         2.567
_exptl_absorpt_coefficient_mu    3.238
_exptl_absorpt_correction_T_max  0.968
_exptl_absorpt_correction_T_min  0.609
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            'dull yellowish green'
_exptl_crystal_colour_lustre     dull
_exptl_crystal_colour_modifier   yellowish
_exptl_crystal_colour_primary    green
_exptl_crystal_density_diffrn    3.073
_exptl_crystal_description       rhombohedral
_exptl_crystal_F_000             2052
_exptl_crystal_size_max          0.23
_exptl_crystal_size_mid          0.13
_exptl_crystal_size_min          0.01
_refine_diff_density_max         0.898
_refine_diff_density_min         -0.849
_refine_diff_density_rms         0.194
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.289
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     376
_refine_ls_number_reflns         4087
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.289
_refine_ls_R_factor_all          0.1021
_refine_ls_R_factor_gt           0.0789
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+64.6160P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1575
_refine_ls_wR_factor_ref         0.1678
_reflns_Friedel_coverage         0.000
_reflns_number_gt                3176
_reflns_number_total             4087
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            ic5b02718_si_004.cif
_cod_data_source_block           sbr105
_cod_database_code               4347093
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_olex2_refinement_description
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H) groups, All N(H) groups
 At 1.5 times of:
  All C(H,H) groups
2. Others
 Fixed Sof: O3(0.5) O16(0.5) O19(0.5) O20(0.5)
 Fixed X: H(WA(0.61904) H(WB(0.57712)
 Fixed Y: H(WA(0.19603) H(WB(0.15007)
 Fixed Z: H(WA(0.035029) H(WB(0.096849)
3.a Aromatic/amide H refined with riding coordinates:
 N1(H1), N2(H2), C2(H2A), C3(H3), C4(H4), C5(H5), C7(H7), C8(H8), C9(H9),
 C10(H10)
;
_shelx_shelxl_version_number     2014/7
_olex2_submission_special_instructions 'No special instructions were received'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, -y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
Mo1 Mo 0.13730(14) 0.74036(12) 0.04403(9) 0.0443(4) Uani 1 1 d . . .
Mo2 Mo 0.17411(14) 1.24471(12) 0.02396(9) 0.0474(4) Uani 1 1 d . . .
Mo3 Mo 0.31122(14) 0.98443(14) 0.07015(9) 0.0500(4) Uani 1 1 d . . .
Mo4 Mo 0.12528(15) 0.92653(15) 0.19885(9) 0.0549(5) Uani 1 1 d . . .
Mo5 Mo -0.01436(17) 1.18624(14) 0.15499(11) 0.0596(5) Uani 1 1 d . . .
Mo6 Mo -0.18690(16) 0.94379(14) 0.13001(11) 0.0577(5) Uani 1 1 d . . .
O1 O 0.1812(13) 0.8968(13) 0.2932(8) 0.083(5) Uani 1 1 d . . .
O2 O 0.0874(13) 1.0866(12) 0.2077(14) 0.118(7) Uani 1 1 d . . .
O3 O -0.002(2) 0.8710(19) -0.0231(13) 0.048(6) Uani 0.5 1 d . . .
O4 O 0.2600(14) 0.9853(13) 0.1684(9) 0.089(5) Uani 1 1 d . . .
O5 O -0.0269(13) 1.2796(12) 0.2229(8) 0.078(4) Uani 1 1 d . . .
O6 O 0.1398(15) 0.7921(14) 0.1513(10) 0.099(6) Uani 1 1 d . . .
O7 O 0.4570(11) 0.9852(11) 0.1046(8) 0.064(4) Uani 1 1 d . . .
O8 O 0.2062(13) 0.6242(11) 0.0700(10) 0.081(5) Uani 1 1 d . . .
O9 O 0.2467(12) 1.3632(11) 0.0301(8) 0.069(4) Uani 1 1 d . . .
O10 O 0.2770(16) 0.8336(12) 0.0550(9) 0.098(6) Uani 1 1 d . . .
O11 O -0.0149(12) 0.7018(16) 0.0354(8) 0.092(5) Uani 1 1 d . . .
O12 O 0.1281(12) 0.7463(14) -0.0619(9) 0.083(5) Uani 1 1 d . . .
O13 O 0.1058(12) 1.2530(16) 0.1136(7) 0.089(5) Uani 1 1 d . . .
O14 O 0.3006(18) 1.0059(14) -0.0386(8) 0.111(7) Uani 1 1 d . . .
O15 O 0.2899(19) 1.1470(14) 0.0758(8) 0.115(7) Uani 1 1 d . . .
O16 O 0.128(2) 1.0592(19) -0.0044(12) 0.045(6) Uani 0.5 1 d . . .
O17 O -0.1913(17) 0.8045(13) 0.0766(8) 0.103(6) Uani 1 1 d . . .
O18 O -0.0383(13) 0.9002(12) 0.1930(14) 0.122(8) Uani 1 1 d . . .
O19 O 0.1070(18) 0.9302(16) 0.0566(12) 0.038(5) Uani 0.5 1 d . . .
O20 O -0.0118(18) 1.0141(18) 0.0924(12) 0.043(5) Uani 0.5 1 d . . .
O21 O -0.2734(12) 0.9141(11) 0.1915(7) 0.065(4) Uani 1 1 d . . .
O22 O -0.1492(13) 1.0942(11) 0.1562(13) 0.109(7) Uani 1 1 d . . .
O(W) O 0.5781(19) 0.2129(13) 0.0709(13) 0.127(8) Uani 1 1 d . . .
N1 N 1.0518(16) 0.594(2) 0.2240(13) 0.092(8) Uani 1 1 d . . .
H1 H 1.1275 0.6023 0.2409 0.111 Uiso 1 1 calc R . .
N2 N 0.4455(15) 0.5331(16) 0.0977(10) 0.071(5) Uani 1 1 d . . .
H2 H 0.3696 0.5238 0.0859 0.085 Uiso 1 1 calc R . .
Si1 Si 0.0000 1.0000 0.0000 0.0376(14) Uani 1 2 d S T P
C1 C 0.8158(18) 0.5724(15) 0.1680(11) 0.055(5) Uani 1 1 d . . .
C2 C 0.8628(17) 0.6472(16) 0.2306(12) 0.060(5) Uani 1 1 d . . .
H2A H 0.8131 0.6918 0.2526 0.073 Uiso 1 1 calc R . .
C3 C 0.8928(19) 0.5077(16) 0.1355(14) 0.069(6) Uani 1 1 d . . .
H3 H 0.8638 0.4564 0.0957 0.083 Uiso 1 1 calc R . .
C4 C 1.012(2) 0.523(2) 0.1644(16) 0.077(7) Uani 1 1 d . . .
H4 H 1.0664 0.4831 0.1428 0.092 Uiso 1 1 calc R . .
C5 C 0.983(2) 0.6509(18) 0.2571(13) 0.067(6) Uani 1 1 d . . .
H5 H 1.0166 0.6956 0.3002 0.081 Uiso 1 1 calc R . .
C6 C 0.6864(17) 0.5586(16) 0.1419(11) 0.055(5) Uani 1 1 d . . .
C7 C 0.6371(15) 0.4552(14) 0.1187(10) 0.048(4) Uani 1 1 d . . .
H7 H 0.6859 0.3942 0.1174 0.058 Uiso 1 1 calc R . .
C8 C 0.5144(17) 0.4447(16) 0.0975(11) 0.058(5) Uani 1 1 d . . .
H8 H 0.4799 0.3759 0.0831 0.069 Uiso 1 1 calc R . .
C9 C 0.4863(18) 0.6328(17) 0.1147(11) 0.059(5) Uani 1 1 d . . .
H9 H 0.4339 0.6921 0.1111 0.071 Uiso 1 1 calc R . .
C10 C 0.6106(16) 0.6503(15) 0.1385(10) 0.051(4) Uani 1 1 d . . .
H10 H 0.6414 0.7208 0.1515 0.061 Uiso 1 1 calc R . .
H(WA H 0.6190 0.1960 0.0350 0.076 Uiso 1 1 d R . .
H(WB H 0.5771 0.1501 0.0968 0.076 Uiso 1 1 d R . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cl Cl 0.1484 0.1585 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O6 Mo1 O3 96.5(8) . .
O6 Mo1 O19 64.4(7) . .
O8 Mo1 O3 161.6(8) . .
O8 Mo1 O6 96.5(8) . .
O8 Mo1 O10 97.6(8) . .
O8 Mo1 O11 101.9(8) . .
O8 Mo1 O12 103.0(8) . .
O8 Mo1 O19 153.6(8) . .
O10 Mo1 O3 96.7(8) . .
O10 Mo1 O6 83.7(6) . .
O10 Mo1 O19 63.8(7) . .
O11 Mo1 O3 65.7(8) . .
O11 Mo1 O6 87.8(7) . .
O11 Mo1 O10 159.5(8) . .
O11 Mo1 O12 95.6(6) . .
O11 Mo1 O19 95.6(8) . .
O12 Mo1 O3 66.5(7) . .
O12 Mo1 O6 159.0(8) . .
O12 Mo1 O10 86.0(6) . .
O12 Mo1 O19 94.6(7) . .
O19 Mo1 O3 44.8(7) . .
O9 Mo2 O3 154.6(8) . 3_575
O9 Mo2 O11 98.3(7) . 3_575
O9 Mo2 O13 101.6(7) . .
O9 Mo2 O15 102.9(8) . .
O9 Mo2 O16 159.4(8) . .
O9 Mo2 O17 100.0(8) . 3_575
O11 Mo2 O3 61.9(7) 3_575 3_575
O11 Mo2 O16 93.8(8) 3_575 .
O13 Mo2 O3 62.8(7) . 3_575
O13 Mo2 O11 84.2(6) . 3_575
O13 Mo2 O16 96.1(8) . .
O15 Mo2 O3 97.6(9) . 3_575
O15 Mo2 O11 158.7(9) . 3_575
O15 Mo2 O13 91.5(7) . .
O15 Mo2 O16 65.9(8) . .
O15 Mo2 O17 91.7(6) . 3_575
O16 Mo2 O3 45.4(8) . 3_575
O17 Mo2 O3 94.1(8) 3_575 3_575
O17 Mo2 O11 84.6(7) 3_575 3_575
O17 Mo2 O13 156.9(8) 3_575 .
O17 Mo2 O16 64.6(7) 3_575 .
O4 Mo3 O15 83.4(7) . .
O4 Mo3 O16 93.6(7) . .
O4 Mo3 O19 66.1(6) . .
O7 Mo3 O4 100.1(7) . .
O7 Mo3 O10 102.8(7) . .
O7 Mo3 O14 100.8(8) . .
O7 Mo3 O15 96.0(8) . .
O7 Mo3 O16 153.5(7) . .
O7 Mo3 O19 158.6(7) . .
O10 Mo3 O4 91.8(6) . .
O10 Mo3 O14 91.8(7) . .
O10 Mo3 O15 161.2(8) . .
O10 Mo3 O16 99.3(8) . .
O10 Mo3 O19 63.3(7) . .
O14 Mo3 O4 157.5(8) . .
O14 Mo3 O15 86.1(6) . .
O14 Mo3 O16 63.8(7) . .
O14 Mo3 O19 95.9(8) . .
O15 Mo3 O16 63.1(8) . .
O15 Mo3 O19 98.3(8) . .
O16 Mo3 O19 47.5(7) . .
O1 Mo4 O2 100.2(9) . .
O1 Mo4 O4 101.5(7) . .
O1 Mo4 O6 101.3(8) . .
O1 Mo4 O18 100.0(9) . .
O1 Mo4 O19 158.8(8) . .
O1 Mo4 O20 154.2(8) . .
O2 Mo4 O19 95.2(8) . .
O2 Mo4 O20 60.8(8) . .
O4 Mo4 O2 82.3(7) . .
O4 Mo4 O18 157.1(8) . .
O4 Mo4 O19 66.1(7) . .
O4 Mo4 O20 93.4(8) . .
O6 Mo4 O2 158.5(9) . .
O6 Mo4 O4 92.4(6) . .
O6 Mo4 O18 91.1(7) . .
O6 Mo4 O19 63.8(7) . .
O6 Mo4 O20 99.1(8) . .
O18 Mo4 O2 86.2(6) . .
O18 Mo4 O19 95.5(9) . .
O18 Mo4 O20 63.7(8) . .
O20 Mo4 O19 47.0(7) . .
O2 Mo5 O3 96.0(9) . 3_575
O2 Mo5 O12 157.1(9) . 3_575
O2 Mo5 O13 91.7(7) . .
O2 Mo5 O20 64.0(8) . .
O2 Mo5 O22 92.5(6) . .
O5 Mo5 O2 104.5(9) . .
O5 Mo5 O3 153.6(7) . 3_575
O5 Mo5 O12 98.4(7) . 3_575
O5 Mo5 O13 99.8(7) . .
O5 Mo5 O20 160.2(8) . .
O5 Mo5 O22 100.6(8) . .
O12 Mo5 O3 62.6(7) 3_575 3_575
O12 Mo5 O20 93.7(7) 3_575 .
O13 Mo5 O3 62.6(7) . 3_575
O13 Mo5 O12 85.5(6) . 3_575
O13 Mo5 O20 96.6(8) . .
O13 Mo5 O22 157.4(8) . .
O20 Mo5 O3 45.9(7) . 3_575
O22 Mo5 O3 94.9(8) . 3_575
O22 Mo5 O12 82.1(7) . 3_575
O22 Mo5 O20 65.6(8) . .
O14 Mo6 O16 62.6(7) 3_575 3_575
O14 Mo6 O17 86.7(6) 3_575 .
O14 Mo6 O20 97.0(8) 3_575 .
O17 Mo6 O16 62.3(7) . 3_575
O17 Mo6 O20 96.3(8) . .
O18 Mo6 O14 158.4(9) . 3_575
O18 Mo6 O16 96.4(9) . 3_575
O18 Mo6 O17 87.3(7) . .
O18 Mo6 O20 63.1(7) . .
O18 Mo6 O22 90.1(7) . .
O20 Mo6 O16 48.6(7) . 3_575
O21 Mo6 O14 101.6(8) . 3_575
O21 Mo6 O16 155.2(7) . 3_575
O21 Mo6 O17 99.6(7) . .
O21 Mo6 O18 99.8(8) . .
O21 Mo6 O20 156.1(7) . .
O21 Mo6 O22 101.1(8) . .
O22 Mo6 O14 88.2(8) . 3_575
O22 Mo6 O16 97.6(8) . 3_575
O22 Mo6 O17 159.3(8) . .
O22 Mo6 O20 64.4(7) . .
Mo5 O2 Mo4 138.2(11) . .
Mo1 O3 Mo2 94.6(8) . 3_575
Mo1 O3 Mo5 94.6(8) . 3_575
Mo2 O3 Mo5 94.1(8) 3_575 3_575
O19 O3 Mo1 66.9(10) . .
O19 O3 Mo2 131.7(12) . 3_575
O19 O3 Mo5 129.9(13) . 3_575
Si1 O3 Mo1 123.7(12) . .
Si1 O3 Mo2 121.9(12) . 3_575
Si1 O3 Mo5 120.5(11) . 3_575
Si1 O3 O19 56.7(10) . .
Mo4 O4 Mo3 133.1(8) . .
Mo4 O6 Mo1 136.3(10) . .
Mo3 O10 Mo1 136.4(10) . .
Mo1 O11 Mo2 136.7(9) . 3_575
Mo1 O12 Mo5 134.8(9) . 3_575
Mo5 O13 Mo2 140.3(10) . .
Mo3 O14 Mo6 138.6(10) . 3_575
Mo2 O15 Mo3 133.7(11) . .
Mo2 O16 Mo3 96.9(8) . .
Mo2 O16 Mo6 96.2(8) . 3_575
Mo3 O16 Mo6 94.9(8) . 3_575
Si1 O16 Mo2 124.5(11) . .
Si1 O16 Mo3 119.9(11) . .
Si1 O16 Mo6 118.1(10) . 3_575
Mo2 O17 Mo6 136.3(9) 3_575 .
Mo6 O18 Mo4 138.4(11) . .
Mo1 O19 Mo3 96.4(7) . .
Mo1 O19 Mo4 95.5(7) . .
Mo3 O19 Mo4 93.0(7) . .
O3 O19 Mo1 68.3(10) . .
O3 O19 Mo3 133.2(12) . .
O3 O19 Mo4 131.1(12) . .
Si1 O19 Mo1 124.2(10) . .
Si1 O19 Mo3 120.6(10) . .
Si1 O19 Mo4 119.9(10) . .
Si1 O19 O3 55.9(10) . .
Mo4 O20 Mo6 94.7(8) . .
Mo5 O20 Mo4 96.5(7) . .
Mo5 O20 Mo6 95.0(8) . .
Si1 O20 Mo4 121.2(11) . .
Si1 O20 Mo5 123.6(12) . .
Si1 O20 Mo6 119.2(10) . .
Mo6 O22 Mo5 134.0(10) . .
H(WA O(W) H(WB 103.4(17) . .
C4 N1 H1 118.1 . .
C5 N1 H1 118.1 . .
C5 N1 C4 124(2) . .
C8 N2 H2 118.0 . .
C9 N2 H2 118.0 . .
C9 N2 C8 124.0(18) . .
O3 Si1 O3 180.0 . 3_575
O3 Si1 O16 68.2(11) 3_575 .
O3 Si1 O16 111.8(11) . .
O3 Si1 O16 111.8(11) 3_575 3_575
O3 Si1 O16 68.2(11) . 3_575
O3 Si1 O19 67.3(10) 3_575 3_575
O3 Si1 O19 112.7(10) . 3_575
O3 Si1 O19 112.7(10) 3_575 .
O3 Si1 O19 67.3(10) . .
O3 Si1 O20 110.0(11) . .
O3 Si1 O20 70.0(11) . 3_575
O3 Si1 O20 110.0(11) 3_575 3_575
O3 Si1 O20 70.0(11) 3_575 .
O16 Si1 O16 180.0 3_575 .
O19 Si1 O16 72.0(10) . .
O19 Si1 O16 72.0(10) 3_575 3_575
O19 Si1 O16 108.0(10) 3_575 .
O19 Si1 O16 108.0(10) . 3_575
O19 Si1 O19 180.0 3_575 .
O19 Si1 O20 71.8(10) 3_575 3_575
O19 Si1 O20 108.2(10) 3_575 .
O19 Si1 O20 71.8(10) . .
O19 Si1 O20 108.2(10) . 3_575
O20 Si1 O16 74.1(10) 3_575 .
O20 Si1 O16 105.9(10) . .
O20 Si1 O16 105.9(10) 3_575 3_575
O20 Si1 O16 74.1(10) . 3_575
O20 Si1 O20 180.0 3_575 .
C2 C1 C6 119.3(18) . .
C3 C1 C2 119.9(19) . .
C3 C1 C6 120.6(18) . .
C1 C2 H2A 121.4 . .
C5 C2 C1 117.3(19) . .
C5 C2 H2A 121.4 . .
C1 C3 H3 121.3 . .
C4 C3 C1 117(2) . .
C4 C3 H3 121.3 . .
N1 C4 C3 120(2) . .
N1 C4 H4 120.0 . .
C3 C4 H4 120.0 . .
N1 C5 C2 121(2) . .
N1 C5 H5 119.3 . .
C2 C5 H5 119.3 . .
C7 C6 C1 120.6(17) . .
C7 C6 C10 119.2(17) . .
C10 C6 C1 120.2(17) . .
C6 C7 H7 120.6 . .
C8 C7 C6 118.8(17) . .
C8 C7 H7 120.6 . .
N2 C8 C7 120.0(18) . .
N2 C8 H8 120.0 . .
C7 C8 H8 120.0 . .
N2 C9 H9 120.2 . .
N2 C9 C10 119.6(19) . .
C10 C9 H9 120.2 . .
C6 C10 C9 118.3(18) . .
C6 C10 H10 120.9 . .
C9 C10 H10 120.9 . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Mo1 O3 2.36(2) .
Mo1 O6 1.954(15) .
Mo1 O8 1.624(13) .
Mo1 O10 1.938(14) .
Mo1 O11 1.788(14) .
Mo1 O12 1.815(14) .
Mo1 O19 2.338(19) .
Mo2 O3 2.42(2) 3_575
Mo2 O9 1.649(13) .
Mo2 O11 1.993(14) 3_575
Mo2 O13 1.898(13) .
Mo2 O15 1.852(15) .
Mo2 O16 2.33(2) .
Mo2 O17 1.894(14) 3_575
Mo3 O4 1.926(13) .
Mo3 O7 1.649(12) .
Mo3 O10 1.870(14) .
Mo3 O14 1.877(14) .
Mo3 O15 1.984(16) .
Mo3 O16 2.38(2) .
Mo3 O19 2.40(2) .
Mo4 O1 1.653(13) .
Mo4 O2 1.997(16) .
Mo4 O4 1.889(13) .
Mo4 O6 1.846(16) .
Mo4 O18 1.892(15) .
Mo4 O19 2.425(19) .
Mo4 O20 2.38(2) .
Mo5 O2 1.779(16) .
Mo5 O3 2.44(2) 3_575
Mo5 O5 1.660(13) .
Mo5 O12 2.002(15) 3_575
Mo5 O13 1.883(14) .
Mo5 O20 2.35(2) .
Mo5 O22 1.915(13) .
Mo6 O14 1.907(15) 3_575
Mo6 O16 2.42(2) 3_575
Mo6 O17 1.915(15) .
Mo6 O18 1.881(17) .
Mo6 O20 2.41(2) .
Mo6 O21 1.658(13) .
Mo6 O22 1.899(14) .
O3 Mo2 2.42(2) 3_575
O3 Mo5 2.44(2) 3_575
O3 O19 1.79(3) .
O3 Si1 1.61(2) .
O11 Mo2 1.993(14) 3_575
O12 Mo5 2.002(15) 3_575
O14 Mo6 1.907(15) 3_575
O16 Mo6 2.42(2) 3_575
O16 Si1 1.66(2) .
O17 Mo2 1.894(14) 3_575
O19 Si1 1.62(2) .
O20 Si1 1.65(2) .
O(W) H(WA 0.885(17) .
O(W) H(WB 0.884(17) .
N1 H1 0.8600 .
N1 C4 1.34(3) .
N1 C5 1.28(3) .
N2 H2 0.8600 .
N2 C8 1.33(2) .
N2 C9 1.30(2) .
Si1 O3 1.61(2) 3_575
Si1 O16 1.66(2) 3_575
Si1 O19 1.62(2) 3_575
Si1 O20 1.65(2) 3_575
C1 C2 1.42(3) .
C1 C3 1.39(3) .
C1 C6 1.47(3) .
C2 H2A 0.9300 .
C2 C5 1.36(3) .
C3 H3 0.9300 .
C3 C4 1.37(3) .
C4 H4 0.9300 .
C5 H5 0.9300 .
C6 C7 1.39(2) .
C6 C10 1.40(2) .
C7 H7 0.9300 .
C7 C8 1.38(2) .
C8 H8 0.9300 .
C9 H9 0.9300 .
C9 C10 1.41(3) .
C10 H10 0.9300 .
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
Mo1 O3 O19 Mo3 78.0(15) . .
Mo1 O3 O19 Mo4 -77.9(14) . .
Mo1 O3 O19 Si1 180.0(10) . .
Mo1 O3 Si1 O16 -121.9(15) . 3_575
Mo1 O3 Si1 O16 58.1(15) . .
Mo1 O3 Si1 O19 180.0(11) . 3_575
Mo1 O3 Si1 O19 0.0(11) . .
Mo1 O3 Si1 O20 -59.3(15) . .
Mo1 O3 Si1 O20 120.7(15) . 3_575
Mo1 O19 Si1 O3 0.0(11) . .
Mo1 O19 Si1 O3 -179.9(11) . 3_575
Mo1 O19 Si1 O16 56.1(14) . 3_575
Mo1 O19 Si1 O16 -123.9(14) . .
Mo1 O19 Si1 O20 -58.1(14) . 3_575
Mo1 O19 Si1 O20 121.9(14) . .
Mo2 O3 O19 Mo1 74.8(15) 3_575 .
Mo2 O3 O19 Mo3 152.8(12) 3_575 .
Mo2 O3 O19 Mo4 -3(3) 3_575 .
Mo2 O3 O19 Si1 -105.2(17) 3_575 .
Mo2 O3 Si1 O16 0.0(11) 3_575 3_575
Mo2 O3 Si1 O16 -180.0(11) 3_575 .
Mo2 O3 Si1 O19 121.9(15) 3_575 .
Mo2 O3 Si1 O19 -58.1(15) 3_575 3_575
Mo2 O3 Si1 O20 -117.3(15) 3_575 3_575
Mo2 O3 Si1 O20 62.7(15) 3_575 .
Mo2 O16 Si1 O3 0.1(11) . 3_575
Mo2 O16 Si1 O3 -179.9(11) . .
Mo2 O16 Si1 O19 -124.5(14) . .
Mo2 O16 Si1 O19 55.5(14) . 3_575
Mo2 O16 Si1 O20 -60.2(14) . .
Mo2 O16 Si1 O20 119.8(14) . 3_575
Mo3 O16 Si1 O3 -55.6(14) . .
Mo3 O16 Si1 O3 124.4(14) . 3_575
Mo3 O16 Si1 O19 -0.1(10) . .
Mo3 O16 Si1 O19 179.9(10) . 3_575
Mo3 O16 Si1 O20 64.2(14) . .
Mo3 O16 Si1 O20 -115.8(14) . 3_575
Mo3 O19 Si1 O3 124.1(14) . .
Mo3 O19 Si1 O3 -55.9(14) . 3_575
Mo3 O19 Si1 O16 -179.9(10) . 3_575
Mo3 O19 Si1 O16 0.1(10) . .
Mo3 O19 Si1 O20 65.9(13) . 3_575
Mo3 O19 Si1 O20 -114.1(13) . .
Mo4 O19 Si1 O3 58.3(14) . 3_575
Mo4 O19 Si1 O3 -121.7(14) . .
Mo4 O19 Si1 O16 114.3(13) . .
Mo4 O19 Si1 O16 -65.7(13) . 3_575
Mo4 O19 Si1 O20 0.1(11) . .
Mo4 O19 Si1 O20 -179.9(11) . 3_575
Mo4 O20 Si1 O3 56.5(15) . .
Mo4 O20 Si1 O3 -123.5(15) . 3_575
Mo4 O20 Si1 O16 115.5(14) . 3_575
Mo4 O20 Si1 O16 -64.5(14) . .
Mo4 O20 Si1 O19 -0.1(11) . .
Mo4 O20 Si1 O19 179.9(11) . 3_575
Mo5 O3 O19 Mo1 -75.9(15) 3_575 .
Mo5 O3 O19 Mo3 2(3) 3_575 .
Mo5 O3 O19 Mo4 -153.8(10) 3_575 .
Mo5 O3 O19 Si1 104.1(16) 3_575 .
Mo5 O3 Si1 O16 -62.2(15) 3_575 .
Mo5 O3 Si1 O16 117.8(15) 3_575 3_575
Mo5 O3 Si1 O19 59.7(15) 3_575 3_575
Mo5 O3 Si1 O19 -120.3(15) 3_575 .
Mo5 O3 Si1 O20 0.5(11) 3_575 3_575
Mo5 O3 Si1 O20 -179.5(11) 3_575 .
Mo5 O20 Si1 O3 -179.5(12) . .
Mo5 O20 Si1 O3 0.5(12) . 3_575
Mo5 O20 Si1 O16 -120.4(14) . 3_575
Mo5 O20 Si1 O16 59.6(14) . .
Mo5 O20 Si1 O19 124.0(14) . .
Mo5 O20 Si1 O19 -56.0(14) . 3_575
Mo6 O16 Si1 O3 -120.9(14) 3_575 3_575
Mo6 O16 Si1 O3 59.1(14) 3_575 .
Mo6 O16 Si1 O19 -65.4(13) 3_575 3_575
Mo6 O16 Si1 O19 114.6(13) 3_575 .
Mo6 O16 Si1 O20 178.9(11) 3_575 .
Mo6 O16 Si1 O20 -1.1(11) 3_575 3_575
Mo6 O20 Si1 O3 119.8(14) . 3_575
Mo6 O20 Si1 O3 -60.2(14) . .
Mo6 O20 Si1 O16 -1.1(11) . 3_575
Mo6 O20 Si1 O16 178.9(11) . .
Mo6 O20 Si1 O19 63.3(14) . 3_575
Mo6 O20 Si1 O19 -116.7(14) . .
O1 Mo4 O4 Mo3 148.2(13) . .
O1 Mo4 O6 Mo1 -162.6(13) . .
O1 Mo4 O18 Mo6 156.5(16) . .
O2 Mo4 O4 Mo3 -112.9(15) . .
O2 Mo4 O6 Mo1 14(3) . .
O2 Mo4 O18 Mo6 56.8(17) . .
O2 Mo5 O13 Mo2 91.1(15) . .
O3 Mo1 O11 Mo2 10.9(12) . 3_575
O3 Mo1 O12 Mo5 -13.0(11) . 3_575
O3 Mo2 O13 Mo5 4.7(13) 3_575 .
O3 Mo2 O15 Mo3 39.5(13) 3_575 .
O3 Mo5 O2 Mo4 -42.2(15) 3_575 .
O3 Mo5 O13 Mo2 -4.7(13) 3_575 .
O3 O19 Si1 O3 180.001(4) . 3_575
O3 O19 Si1 O16 56.0(12) . 3_575
O3 O19 Si1 O16 -124.0(12) . .
O3 O19 Si1 O20 -58.2(12) . 3_575
O3 O19 Si1 O20 121.8(12) . .
O4 Mo3 O10 Mo1 59.6(13) . .
O4 Mo3 O14 Mo6 -1(3) . 3_575
O4 Mo4 O6 Mo1 -60.4(14) . .
O4 Mo4 O18 Mo6 -3(3) . .
O5 Mo5 O2 Mo4 154.5(14) . .
O5 Mo5 O13 Mo2 -163.8(14) . .
O6 Mo1 O11 Mo2 109.1(14) . 3_575
O6 Mo1 O12 Mo5 -51(2) . 3_575
O6 Mo4 O4 Mo3 46.2(14) . .
O6 Mo4 O18 Mo6 -101.9(17) . .
O7 Mo3 O10 Mo1 160.3(12) . .
O7 Mo3 O14 Mo6 -158.9(15) . 3_575
O8 Mo1 O11 Mo2 -154.7(13) . 3_575
O8 Mo1 O12 Mo5 150.9(11) . 3_575
O9 Mo2 O13 Mo5 163.4(13) . .
O9 Mo2 O15 Mo3 -155.5(12) . .
O10 Mo1 O11 Mo2 44(3) . 3_575
O10 Mo1 O12 Mo5 -112.1(12) . 3_575
O10 Mo3 O14 Mo6 97.7(16) . 3_575
O11 Mo1 O12 Mo5 47.4(13) . 3_575
O11 Mo2 O13 Mo5 66.1(14) 3_575 .
O11 Mo2 O15 Mo3 25(3) 3_575 .
O12 Mo1 O11 Mo2 -50.1(14) . 3_575
O12 Mo5 O2 Mo4 -22(3) 3_575 .
O12 Mo5 O13 Mo2 -66.1(14) 3_575 .
O13 Mo2 O15 Mo3 102.3(13) . .
O13 Mo5 O2 Mo4 -104.9(15) . .
O14 Mo3 O10 Mo1 -98.2(13) . .
O14 Mo6 O18 Mo4 27(3) 3_575 .
O14 Mo6 O22 Mo5 -108.9(15) 3_575 .
O15 Mo2 O13 Mo5 -93.0(15) . .
O15 Mo3 O10 Mo1 -15(3) . .
O15 Mo3 O14 Mo6 -63.6(16) . 3_575
O16 Mo2 O13 Mo5 -27.1(15) . .
O16 Mo2 O15 Mo3 6.2(11) . .
O16 Mo3 O10 Mo1 -34.4(13) . .
O16 Mo3 O14 Mo6 -1.8(14) . 3_575
O16 Mo6 O18 Mo4 39.0(17) 3_575 .
O16 Mo6 O22 Mo5 -46.8(16) 3_575 .
O17 Mo2 O13 Mo5 5(3) 3_575 .
O17 Mo2 O15 Mo3 -54.8(14) 3_575 .
O17 Mo6 O18 Mo4 100.7(17) . .
O17 Mo6 O22 Mo5 -33(3) . .
O18 Mo4 O4 Mo3 -52(3) . .
O18 Mo4 O6 Mo1 97.0(14) . .
O18 Mo6 O22 Mo5 49.7(16) . .
O19 Mo1 O11 Mo2 45.1(14) . 3_575
O19 Mo1 O12 Mo5 -48.8(12) . 3_575
O19 Mo3 O10 Mo1 -2.4(11) . .
O19 Mo3 O14 Mo6 34.4(17) . 3_575
O19 Mo4 O4 Mo3 -13.7(12) . .
O19 Mo4 O6 Mo1 1.4(11) . .
O19 Mo4 O18 Mo6 -38.1(17) . .
O19 O3 Si1 O16 58.1(12) . .
O19 O3 Si1 O16 -121.9(12) . 3_575
O19 O3 Si1 O19 180.000(5) . 3_575
O19 O3 Si1 O20 -59.2(12) . .
O19 O3 Si1 O20 120.8(12) . 3_575
O20 Mo4 O4 Mo3 -53.1(14) . .
O20 Mo4 O6 Mo1 33.4(14) . .
O20 Mo4 O18 Mo6 -2.3(14) . .
O20 Mo5 O2 Mo4 -8.3(13) . .
O20 Mo5 O13 Mo2 27.2(15) . .
O20 Mo6 O18 Mo4 2.3(14) . .
O20 Mo6 O22 Mo5 -10.2(13) . .
O21 Mo6 O18 Mo4 -160.0(16) . .
O21 Mo6 O22 Mo5 149.6(14) . .
O22 Mo5 O2 Mo4 52.9(16) . .
O22 Mo5 O13 Mo2 -9(3) . .
O22 Mo6 O18 Mo4 -58.7(17) . .
N2 C9 C10 C6 1(3) . .
Si1 O3 O19 Mo1 -180.0(10) . .
Si1 O3 O19 Mo3 -102.0(16) . .
Si1 O3 O19 Mo4 102.1(15) . .
C1 C2 C5 N1 4(3) . .
C1 C3 C4 N1 3(3) . .
C1 C6 C7 C8 177.5(17) . .
C1 C6 C10 C9 -178.6(16) . .
C2 C1 C3 C4 -2(3) . .
C2 C1 C6 C7 -143.2(18) . .
C2 C1 C6 C10 38(3) . .
C3 C1 C2 C5 -1(3) . .
C3 C1 C6 C7 33(3) . .
C3 C1 C6 C10 -146.0(19) . .
C4 N1 C5 C2 -4(3) . .
C5 N1 C4 C3 0(3) . .
C6 C1 C2 C5 174.9(18) . .
C6 C1 C3 C4 -177.9(18) . .
C6 C7 C8 N2 2(3) . .
C7 C6 C10 C9 3(3) . .
C8 N2 C9 C10 -3(3) . .
C9 N2 C8 C7 2(3) . .
C10 C6 C7 C8 -4(3) . .
